Solid-State Synthesis and Characterization of Novel Aluminophosphates, A3Al2P3O12 (A = Na, K, Rb, Tl): Influence of A+ Ions on the Coordination of Aluminum
R. Nandini Devi; K. Vidyasagar; Inorganic Chemistry 39 (2000) 2391–2396; doi:10.1021/ic991395u

data_4320993
_publ_section_title
;
 Solid-State Synthesis and Characterization of Novel Aluminophosphates,
 A3Al2P3O12 (A = Na, K, Rb, Tl): Influence of A+ Ions on the Coordination
 of Aluminum
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2391
_journal_page_last               2396
_journal_paper_doi               10.1021/ic991395u
_journal_volume                  39
_journal_year                    2000
_chemical_formula_sum            'Al2 K3 O12 P3'
_chemical_formula_weight         456.09
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           33
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  'P 2c -2n'
_symmetry_space_group_name_H-M   'P n a 21'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   8.685(2)
_cell_length_b                   16.947(2)
_cell_length_c                   8.458(3)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      15
_cell_measurement_theta_min      10
_cell_volume                     1244.9(5)
_computing_cell_refinement       'CAD4 programs'
_computing_data_collection       'CAD4 programs'
_computing_data_reduction        MoLEN
_computing_molecular_graphics    ORTEP92
_computing_publication_material  'SHELXL-93 (Sheldrick, 1993)'
_computing_structure_refinement  'SHELXL-93 (Sheldrick, 1993)'
_computing_structure_solution    'SHELXS-86 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measurement_device       'Enraf Nonius CAD4'
_diffrn_measurement_method       2theta-omega
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0208
_diffrn_reflns_av_sigmaI/netI    0.0236
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            1177
_diffrn_reflns_theta_max         24.95
_diffrn_reflns_theta_min         2.40
_diffrn_standards_decay_%        2%
_diffrn_standards_interval_time  '1 hour'
_diffrn_standards_number         2
_exptl_absorpt_coefficient_mu    1.598
_exptl_absorpt_correction_T_max  0.999
_exptl_absorpt_correction_T_min  0.889
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.434
_exptl_crystal_description       'rectangular blockshaped'
_exptl_crystal_F_000             896
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.15
_refine_diff_density_max         0.342
_refine_diff_density_min         -0.328
_refine_diff_density_rms         0.074
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.03(6)
_refine_ls_extinction_coef       0.0073(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_all   1.098
_refine_ls_goodness_of_fit_obs   1.089
_refine_ls_matrix_type           full
_refine_ls_number_parameters     182
_refine_ls_number_reflns         1176
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.097
_refine_ls_restrained_S_obs      1.088
_refine_ls_R_factor_all          0.0261
_refine_ls_R_factor_obs          0.0233
_refine_ls_shift/esd_max         0.001
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0343P)^2^+0.6698P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.0597
_refine_ls_wR_factor_obs         0.0575
_reflns_number_observed          1117
_reflns_number_total             1176
_reflns_observed_criterion       >2sigma(I)
_cod_data_source_file            ic991395u_1.cif
_cod_data_source_block           K3Al2P3O12
_cod_depositor_comments
;
The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc
w=1/[\s^2^(Fo^2^)+(0.0343P)^2^+0.6698P] where P=(Fo^2^+2Fc^2^)/3' was
changed to 'calc'. New tag '_refine_ls_weighting_details' was
created. The value of the new tag was set to
'w=1/[\s^2^(Fo^2^)+(0.0343P)^2^+0.6698P] where P=(Fo^2^+2Fc^2^)/3'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_database_code               4320993